#------------------------------------------------------------------------------
#$Date: 2016-03-23 22:00:51 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179462 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/59/4335910.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4335910
loop_
_publ_author_name
'Nicholas P. Calta'
'Mercouri G. Kanatzidis'
_publ_section_title
;
 Quaternary Aluminum Silicides Grown in Al Flux: RE5Mn4Al23-xSix (RE = Ho,
 Er, Yb) and Er44Mn55(AlSi)237
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              9931
_journal_page_last               9940
_journal_paper_doi               10.1021/ic401659y
_journal_volume                  52
_journal_year                    2013
_chemical_formula_sum            'Al236 Er88 Mn110 Si238'
_chemical_formula_weight         33814.98
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           223
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-P 4n 2 3'
_symmetry_space_group_name_H-M   'P m -3 n'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   21.8208(4)
_cell_length_b                   21.8208(4)
_cell_length_c                   21.8208(4)
_cell_measurement_reflns_used    30886
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      28.48
_cell_measurement_theta_min      1.86
_cell_volume                     10389.9(3)
_computing_cell_refinement       'STOE X-AREA'
_computing_data_collection       'STOE X-AREA'
_computing_data_reduction        'STOE X-RED'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector                 'image plate (34 cm diameter)'
_diffrn_detector_area_resol_mean 6.67
_diffrn_detector_type            STOE
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device       '2-circle goniometer'
_diffrn_measurement_device_type  'STOE IPDS 2'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1166
_diffrn_reflns_av_sigmaI/netI    0.0239
_diffrn_reflns_limit_h_max       25
_diffrn_reflns_limit_h_min       -25
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            56227
_diffrn_reflns_theta_full        24.99
_diffrn_reflns_theta_max         24.99
_diffrn_reflns_theta_min         1.87
_exptl_absorpt_coefficient_mu    21.960
_exptl_absorpt_correction_T_max  0.4918
_exptl_absorpt_correction_T_min  0.3082
_exptl_absorpt_correction_type   integration
_exptl_absorpt_process_details   X-Red32
_exptl_crystal_colour            'metallic silver'
_exptl_crystal_density_diffrn    5.404
_exptl_crystal_description       plate
_exptl_crystal_F_000             15134
_exptl_crystal_size_max          0.061
_exptl_crystal_size_mid          0.045
_exptl_crystal_size_min          0.002
_refine_diff_density_max         1.312
_refine_diff_density_min         -1.712
_refine_diff_density_rms         0.273
_refine_ls_extinction_coef       0.000014(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.445
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     149
_refine_ls_number_reflns         1661
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.445
_refine_ls_R_factor_all          0.0603
_refine_ls_R_factor_gt           0.0502
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0175P)²+232.5937P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0712
_refine_ls_wR_factor_ref         0.0730
_reflns_number_gt                1510
_reflns_number_total             1661
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic401659y_si_001_1.cif
_cod_data_source_block           cubic
_cod_database_code               4335910
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y+1/2, x+1/2, -z+1/2'
'-y+1/2, -x+1/2, -z+1/2'
'y+1/2, -x+1/2, z+1/2'
'-y+1/2, x+1/2, z+1/2'
'x+1/2, z+1/2, -y+1/2'
'-x+1/2, z+1/2, y+1/2'
'-x+1/2, -z+1/2, -y+1/2'
'x+1/2, -z+1/2, y+1/2'
'z+1/2, y+1/2, -x+1/2'
'z+1/2, -y+1/2, x+1/2'
'-z+1/2, y+1/2, x+1/2'
'-z+1/2, -y+1/2, -x+1/2'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-z, -x, -y'
'-z, x, y'
'z, x, -y'
'z, -x, y'
'-y, -z, -x'
'y, -z, x'
'-y, z, x'
'y, z, -x'
'-y-1/2, -x-1/2, z-1/2'
'y-1/2, x-1/2, z-1/2'
'-y-1/2, x-1/2, -z-1/2'
'y-1/2, -x-1/2, -z-1/2'
'-x-1/2, -z-1/2, y-1/2'
'x-1/2, -z-1/2, -y-1/2'
'x-1/2, z-1/2, y-1/2'
'-x-1/2, z-1/2, -y-1/2'
'-z-1/2, -y-1/2, x-1/2'
'-z-1/2, y-1/2, -x-1/2'
'z-1/2, -y-1/2, -x-1/2'
'z-1/2, y-1/2, x-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Er1 Er 0.0000 0.22038(4) 0.29116(4) 0.0063(2) Uani 1 2 d S
Er2 Er 0.0000 0.36256(4) 0.40809(4) 0.0081(2) Uani 1 2 d S
Er3 Er 0.0000 0.37048(4) 0.08653(4) 0.0075(2) Uani 1 2 d S
Er4 Er 0.09152(3) 0.09152(3) 0.09152(3) 0.0074(2) Uani 1 3 d S
Mn1 Mn 0.09594(8) 0.10966(8) 0.24689(9) 0.0047(4) Uani 1 1 d .
Mn2 Mn 0.0000 0.36286(13) 0.25413(13) 0.0079(6) Uani 1 2 d S
Mn4 Mn 0.2500 0.2500 0.2500 0.0053(8) Uani 1 6 d S
Mn3 Mn 0.2500 0.60336(9) 0.10336(9) 0.0056(5) Uani 1 2 d S
Mn5 Mn 0.0000 0.5000 0.5000 0.0072(11) Uani 1 8 d S
Al1 Al 0.06319(17) 0.43445(18) 0.19164(17) 0.0094(7) Uani 0.50 1 d P
Si1 Si 0.06319(17) 0.43445(18) 0.19164(17) 0.0094(7) Uani 0.50 1 d P
Al2 Al 0.06341(18) 0.19197(17) 0.17943(16) 0.0075(8) Uani 0.50 1 d P
Si2 Si 0.06341(18) 0.19197(17) 0.17943(16) 0.0075(8) Uani 0.50 1 d P
Al3 Al 0.07253(18) 0.30716(18) 0.18900(19) 0.0117(8) Uani 0.50 1 d P
Si3 Si 0.07253(18) 0.30716(18) 0.18900(19) 0.0117(8) Uani 0.50 1 d P
Al4 Al 0.08273(16) 0.31798(16) 0.31094(16) 0.0033(7) Uani 0.50 1 d P
Si4 Si 0.08273(16) 0.31798(16) 0.31094(16) 0.0033(7) Uani 0.50 1 d P
Al5 Al 0.08836(18) 0.13807(18) 0.36193(18) 0.0107(8) Uani 0.50 1 d P
Si5 Si 0.08836(18) 0.13807(18) 0.36193(18) 0.0107(8) Uani 0.50 1 d P
Al6 Al 0.14212(17) 0.21264(19) 0.28709(19) 0.0121(8) Uani 0.50 1 d P
Si6 Si 0.14212(17) 0.21264(19) 0.28709(19) 0.0121(8) Uani 0.50 1 d P
Al7 Al 0.0000 0.0793(2) 0.3015(2) 0.0069(11) Uani 0.50 2 d SP
Si7 Si 0.0000 0.0793(2) 0.3015(2) 0.0069(11) Uani 0.50 2 d SP
Al8 Al 0.0000 0.0847(2) 0.4222(2) 0.0063(10) Uani 0.50 2 d SP
Si8 Si 0.0000 0.0847(2) 0.4222(2) 0.0063(10) Uani 0.50 2 d SP
Al9 Al 0.0000 0.0960(3) 0.1901(2) 0.0070(10) Uani 0.50 2 d SP
Si9 Si 0.0000 0.0960(3) 0.1901(2) 0.0070(10) Uani 0.50 2 d SP
Al10 Al 0.0000 0.2171(3) 0.4252(2) 0.0098(11) Uani 0.50 2 d SP
Si10 Si 0.0000 0.2171(3) 0.4252(2) 0.0098(11) Uani 0.50 2 d SP
Al11 Al 0.0000 0.2216(3) 0.0798(3) 0.0131(12) Uani 0.50 2 d SP
Si11 Si 0.0000 0.2216(3) 0.0798(3) 0.0131(12) Uani 0.50 2 d SP
Al12 Al 0.2500 0.17451(15) 0.67451(15) 0.0043(10) Uani 0.50 2 d SP
Si12 Si 0.2500 0.17451(15) 0.67451(15) 0.0043(10) Uani 0.50 2 d SP
Al13 Al 0.17792(19) 0.17792(19) 0.17792(19) 0.0150(14) Uani 0.50 3 d SP
Si13 Si 0.17792(19) 0.17792(19) 0.17792(19) 0.0150(14) Uani 0.50 3 d SP
Al14 Al 0.1117(3) 0.0000 0.5000 0.0032(14) Uani 0.50 4 d SP
Si14 Si 0.1117(3) 0.0000 0.5000 0.0032(14) Uani 0.50 4 d SP
Al15 Al 0.1255(3) 0.0000 0.0000 0.0052(14) Uani 0.50 4 d SP
Si15 Si 0.1255(3) 0.0000 0.0000 0.0052(14) Uani 0.50 4 d SP
Al16 Al 0.0000 0.0000 0.0000 0.004(3) Uani 0.50 24 d SP
Si16 Si 0.0000 0.0000 0.0000 0.004(3) Uani 0.50 24 d SP
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Er Er -0.2586 4.9576 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Al4 Er1 Si4 79.43(14) . 28
Al4 Er1 Al4 79.43(14) . 28
Si4 Er1 Al4 0.00(18) 28 28
Al4 Er1 Al2 89.11(10) . .
Si4 Er1 Al2 126.90(11) 28 .
Al4 Er1 Al2 126.90(11) 28 .
Al4 Er1 Si2 126.90(11) . 28
Si4 Er1 Si2 89.11(10) 28 28
Al4 Er1 Si2 89.11(10) 28 28
Al2 Er1 Si2 57.62(15) . 28
Al4 Er1 Al2 126.90(11) . 28
Si4 Er1 Al2 89.11(10) 28 28
Al4 Er1 Al2 89.11(10) 28 28
Al2 Er1 Al2 57.62(15) . 28
Si2 Er1 Al2 0.0(2) 28 28
Al4 Er1 Al10 82.27(12) . .
Si4 Er1 Al10 82.28(12) 28 .
Al4 Er1 Al10 82.28(12) 28 .
Al2 Er1 Al10 147.53(10) . .
Si2 Er1 Al10 147.54(10) 28 .
Al2 Er1 Al10 147.54(10) 28 .
Al4 Er1 Si5 140.31(11) . 28
Si4 Er1 Si5 87.86(10) 28 28
Al4 Er1 Si5 87.86(10) 28 28
Al2 Er1 Si5 127.34(11) . 28
Si2 Er1 Si5 89.89(11) 28 28
Al2 Er1 Si5 89.89(11) 28 28
Al10 Er1 Si5 58.69(11) . 28
Al4 Er1 Al5 140.31(11) . 28
Si4 Er1 Al5 87.86(10) 28 28
Al4 Er1 Al5 87.86(10) 28 28
Al2 Er1 Al5 127.34(11) . 28
Si2 Er1 Al5 89.89(11) 28 28
Al2 Er1 Al5 89.89(11) 28 28
Al10 Er1 Al5 58.69(11) . 28
Si5 Er1 Al5 0.00(16) 28 28
Si8 Er2 Al8 0.0 45_666 45_666
Si8 Er2 Si8 72.54(17) 45_666 22_455
Al8 Er2 Si8 72.54(17) 45_666 22_455
Si8 Er2 Al8 72.54(17) 45_666 22_455
Al8 Er2 Al8 72.54(17) 45_666 22_455
Si8 Er2 Al8 0.00(16) 22_455 22_455
Si8 Er2 Al4 105.83(11) 45_666 .
Al8 Er2 Al4 105.83(11) 45_666 .
Si8 Er2 Al4 175.59(12) 22_455 .
Al8 Er2 Al4 175.59(12) 22_455 .
Si8 Er2 Si4 175.59(12) 45_666 28
Al8 Er2 Si4 175.59(12) 45_666 28
Si8 Er2 Si4 105.83(11) 22_455 28
Al8 Er2 Si4 105.83(11) 22_455 28
Al4 Er2 Si4 75.48(14) . 28
Si8 Er2 Al4 175.59(12) 45_666 28
Al8 Er2 Al4 175.59(12) 45_666 28
Si8 Er2 Al4 105.83(11) 22_455 28
Al8 Er2 Al4 105.83(11) 22_455 28
Al4 Er2 Al4 75.48(14) . 28
Si4 Er2 Al4 0.00(16) 28 28
Si8 Er2 Si5 52.59(11) 45_666 24
Al8 Er2 Si5 52.59(11) 45_666 24
Si8 Er2 Si5 125.12(12) 22_455 24
Al8 Er2 Si5 125.12(12) 22_455 24
Al4 Er2 Si5 53.49(10) . 24
Si4 Er2 Si5 128.96(10) 28 24
Al4 Er2 Si5 128.96(10) 28 24
Si8 Er2 Al5 52.59(11) 45_666 24
Al8 Er2 Al5 52.59(11) 45_666 24
Si8 Er2 Al5 125.12(12) 22_455 24
Al8 Er2 Al5 125.12(12) 22_455 24
Al4 Er2 Al5 53.49(10) . 24
Si4 Er2 Al5 128.96(10) 28 24
Al4 Er2 Al5 128.96(10) 28 24
Si5 Er2 Al5 0.0(2) 24 24
Si8 Er2 Si5 125.12(12) 45_666 47_566
Al8 Er2 Si5 125.12(12) 45_666 47_566
Si8 Er2 Si5 52.59(11) 22_455 47_566
Al8 Er2 Si5 52.59(11) 22_455 47_566
Al4 Er2 Si5 128.96(10) . 47_566
Si4 Er2 Si5 53.49(10) 28 47_566
Al4 Er2 Si5 53.49(10) 28 47_566
Si5 Er2 Si5 177.01(15) 24 47_566
Al5 Er2 Si5 177.01(15) 24 47_566
Si8 Er2 Al5 125.12(12) 45_666 47_566
Al8 Er2 Al5 125.12(12) 45_666 47_566
Si8 Er2 Al5 52.59(11) 22_455 47_566
Al8 Er2 Al5 52.59(11) 22_455 47_566
Al4 Er2 Al5 128.96(10) . 47_566
Si4 Er2 Al5 53.49(10) 28 47_566
Al4 Er2 Al5 53.49(10) 28 47_566
Si5 Er2 Al5 177.01(15) 24 47_566
Al5 Er2 Al5 177.01(15) 24 47_566
Si5 Er2 Al5 0.00(15) 47_566 47_566
Si8 Er3 Al8 0.0(2) 10 10
Si8 Er3 Si8 80.05(18) 10 9
Al8 Er3 Si8 80.05(18) 10 9
Si8 Er3 Al8 80.05(18) 10 9
Al8 Er3 Al8 80.05(18) 10 9
Si8 Er3 Al8 0.00(18) 9 9
Si8 Er3 Si14 74.92(14) 10 9
Al8 Er3 Si14 74.92(14) 10 9
Si8 Er3 Si14 74.92(14) 9 9
Al8 Er3 Si14 74.92(14) 9 9
Si8 Er3 Al14 74.92(14) 10 9
Al8 Er3 Al14 74.92(14) 10 9
Si8 Er3 Al14 74.92(14) 9 9
Al8 Er3 Al14 74.92(14) 9 9
Si14 Er3 Al14 0.0(3) 9 9
Si8 Er3 Si7 53.62(13) 10 10
Al8 Er3 Si7 53.62(13) 10 10
Si8 Er3 Si7 98.99(10) 9 10
Al8 Er3 Si7 98.99(10) 9 10
Si14 Er3 Si7 128.23(13) 9 10
Al14 Er3 Si7 128.23(13) 9 10
Si8 Er3 Al7 53.62(13) 10 10
Al8 Er3 Al7 53.62(13) 10 10
Si8 Er3 Al7 98.99(10) 9 10
Al8 Er3 Al7 98.99(10) 9 10
Si14 Er3 Al7 128.23(13) 9 10
Al14 Er3 Al7 128.23(13) 9 10
Si7 Er3 Al7 0.0(2) 10 10
Si8 Er3 Si7 98.99(10) 10 9
Al8 Er3 Si7 98.99(10) 10 9
Si8 Er3 Si7 53.62(13) 9 9
Al8 Er3 Si7 53.62(13) 9 9
Si14 Er3 Si7 128.23(13) 9 9
Al14 Er3 Si7 128.23(13) 9 9
Si7 Er3 Si7 71.27(18) 10 9
Al7 Er3 Si7 71.27(18) 10 9
Si8 Er3 Al7 98.99(10) 10 9
Al8 Er3 Al7 98.99(10) 10 9
Si8 Er3 Al7 53.62(13) 9 9
Al8 Er3 Al7 53.62(13) 9 9
Si14 Er3 Al7 128.23(13) 9 9
Al14 Er3 Al7 128.23(13) 9 9
Si7 Er3 Al7 71.27(18) 10 9
Al7 Er3 Al7 71.27(18) 10 9
Si7 Er3 Al7 0.0(2) 9 9
Si8 Er3 Al1 91.36(10) 10 28
Al8 Er3 Al1 91.36(10) 10 28
Si8 Er3 Al1 127.69(12) 9 28
Al8 Er3 Al1 127.69(12) 9 28
Si14 Er3 Al1 53.19(13) 9 28
Al14 Er3 Al1 53.19(13) 9 28
Si7 Er3 Al1 116.81(11) 10 28
Al7 Er3 Al1 116.81(11) 10 28
Si7 Er3 Al1 169.54(10) 9 28
Al7 Er3 Al1 169.54(10) 9 28
Si8 Er3 Si1 91.36(10) 10 28
Al8 Er3 Si1 91.36(10) 10 28
Si8 Er3 Si1 127.69(12) 9 28
Al8 Er3 Si1 127.69(12) 9 28
Si14 Er3 Si1 53.19(13) 9 28
Al14 Er3 Si1 53.19(13) 9 28
Si7 Er3 Si1 116.81(11) 10 28
Al7 Er3 Si1 116.81(11) 10 28
Si7 Er3 Si1 169.54(10) 9 28
Al7 Er3 Si1 169.54(10) 9 28
Al1 Er3 Si1 0.00(16) 28 28
Si15 Er4 Si15 83.1(2) 9 5
Si15 Er4 Al15 0.0(3) 9 9
Si15 Er4 Al15 83.1(2) 5 9
Si15 Er4 Al15 83.1(2) 9 5
Si15 Er4 Al15 0.0(3) 5 5
Al15 Er4 Al15 83.1(2) 9 5
Si15 Er4 Al15 83.1(2) 9 .
Si15 Er4 Al15 83.1(2) 5 .
Al15 Er4 Al15 83.1(2) 9 .
Al15 Er4 Al15 83.1(2) 5 .
Si15 Er4 Si9 134.14(15) 9 9
Si15 Er4 Si9 51.05(15) 5 9
Al15 Er4 Si9 134.14(15) 9 9
Al15 Er4 Si9 51.05(15) 5 9
Al15 Er4 Si9 91.57(7) . 9
Si15 Er4 Si9 91.57(7) 9 5
Si15 Er4 Si9 134.14(15) 5 5
Al15 Er4 Si9 91.57(7) 9 5
Al15 Er4 Si9 134.14(15) 5 5
Al15 Er4 Si9 51.05(15) . 5
Si9 Er4 Si9 119.759(15) 9 5
Si15 Er4 Al9 134.14(15) 9 9
Si15 Er4 Al9 51.05(15) 5 9
Al15 Er4 Al9 134.14(15) 9 9
Al15 Er4 Al9 51.05(15) 5 9
Al15 Er4 Al9 91.57(7) . 9
Si9 Er4 Al9 0.00(14) 9 9
Si9 Er4 Al9 119.759(15) 5 9
Si15 Er4 Al9 91.57(7) 9 5
Si15 Er4 Al9 134.14(15) 5 5
Al15 Er4 Al9 91.57(7) 9 5
Al15 Er4 Al9 134.14(15) 5 5
Al15 Er4 Al9 51.05(15) . 5
Si9 Er4 Al9 119.759(15) 9 5
Si9 Er4 Al9 0.0(3) 5 5
Al9 Er4 Al9 119.759(15) 9 5
Si15 Er4 Al9 51.05(15) 9 .
Si15 Er4 Al9 91.56(7) 5 .
Al15 Er4 Al9 51.05(15) 9 .
Al15 Er4 Al9 91.56(7) 5 .
Al15 Er4 Al9 134.14(15) . .
Si9 Er4 Al9 119.758(15) 9 .
Si9 Er4 Al9 119.760(15) 5 .
Al9 Er4 Al9 119.758(15) 9 .
Al9 Er4 Al9 119.760(15) 5 .
Si2 Mn1 Al2 0.0(2) 5 5
Si2 Mn1 Al2 103.30(18) 5 .
Al2 Mn1 Al2 103.30(18) 5 .
Si2 Mn1 Al9 110.13(16) 5 .
Al2 Mn1 Al9 110.13(16) 5 .
Al2 Mn1 Al9 62.21(16) . .
Si2 Mn1 Si11 65.91(17) 5 5
Al2 Mn1 Si11 65.91(17) 5 5
Al2 Mn1 Si11 122.48(18) . 5
Al9 Mn1 Si11 69.43(19) . 5
Si2 Mn1 Al11 65.91(17) 5 5
Al2 Mn1 Al11 65.91(17) 5 5
Al2 Mn1 Al11 122.48(18) . 5
Al9 Mn1 Al11 69.43(19) . 5
Si11 Mn1 Al11 0.0(4) 5 5
Si2 Mn1 Al7 139.64(17) 5 .
Al2 Mn1 Al7 139.64(17) 5 .
Al2 Mn1 Al7 103.89(16) . .
Al9 Mn1 Al7 59.54(15) . .
Si11 Mn1 Al7 74.41(19) 5 .
Al11 Mn1 Al7 74.41(19) 5 .
Si2 Mn1 Si3 61.33(12) 5 5
Al2 Mn1 Si3 61.33(12) 5 5
Al2 Mn1 Si3 141.27(14) . 5
Al9 Mn1 Si3 154.39(18) . 5
Si11 Mn1 Si3 85.50(17) 5 5
Al11 Mn1 Si3 85.50(17) 5 5
Al7 Mn1 Si3 109.69(15) . 5
Si2 Mn1 Al3 61.33(12) 5 5
Al2 Mn1 Al3 61.33(12) 5 5
Al2 Mn1 Al3 141.27(14) . 5
Al9 Mn1 Al3 154.39(18) . 5
Si11 Mn1 Al3 85.50(17) 5 5
Al11 Mn1 Al3 85.50(17) 5 5
Al7 Mn1 Al3 109.69(15) . 5
Si3 Mn1 Al3 0.0(2) 5 5
Al4 Mn2 Si4 97.6(2) . 28
Al4 Mn2 Al4 97.6(2) . 28
Si4 Mn2 Al4 0.00(18) 28 28
Al4 Mn2 Si3 125.69(17) . 28
Si4 Mn2 Si3 67.12(12) 28 28
Al4 Mn2 Si3 67.12(12) 28 28
Al4 Mn2 Al3 125.69(17) . 28
Si4 Mn2 Al3 67.12(12) 28 28
Al4 Mn2 Al3 67.12(12) 28 28
Si3 Mn2 Al3 0.0(3) 28 28
Al4 Mn2 Al3 67.12(12) . .
Si4 Mn2 Al3 125.69(17) 28 .
Al4 Mn2 Al3 125.69(17) 28 .
Si3 Mn2 Al3 80.5(2) 28 .
Al3 Mn2 Al3 80.5(2) 28 .
Al4 Mn2 Si1 65.27(13) . 14
Si4 Mn2 Si1 117.18(17) 28 14
Al4 Mn2 Si1 117.18(17) 28 14
Si3 Mn2 Si1 168.59(17) 28 14
Al3 Mn2 Si1 168.59(17) 28 14
Al3 Mn2 Si1 103.24(13) . 14
Al4 Mn2 Al1 65.27(13) . 14
Si4 Mn2 Al1 117.18(17) 28 14
Al4 Mn2 Al1 117.18(17) 28 14
Si3 Mn2 Al1 168.59(17) 28 14
Al3 Mn2 Al1 168.59(17) 28 14
Al3 Mn2 Al1 103.24(13) . 14
Si1 Mn2 Al1 0.0(2) 14 14
Al4 Mn2 Si1 117.17(17) . 40_566
Si4 Mn2 Si1 65.26(13) 28 40_566
Al4 Mn2 Si1 65.26(13) 28 40_566
Si3 Mn2 Si1 103.24(13) 28 40_566
Al3 Mn2 Si1 103.24(13) 28 40_566
Al3 Mn2 Si1 168.59(17) . 40_566
Si1 Mn2 Si1 71.11(19) 14 40_566
Al1 Mn2 Si1 71.11(19) 14 40_566
Al4 Mn2 Al1 117.17(17) . 40_566
Si4 Mn2 Al1 65.26(13) 28 40_566
Al4 Mn2 Al1 65.26(13) 28 40_566
Si3 Mn2 Al1 103.24(13) 28 40_566
Al3 Mn2 Al1 103.24(13) 28 40_566
Al3 Mn2 Al1 168.59(17) . 40_566
Si1 Mn2 Al1 71.11(19) 14 40_566
Al1 Mn2 Al1 71.11(19) 14 40_566
Si1 Mn2 Al1 0.0(2) 40_566 40_566
Si12 Mn4 Si12 120.0 34_565 30_655
Si12 Mn4 Si12 120.0 34_565 26_556
Si12 Mn4 Si12 120.0 30_655 26_556
Si12 Mn4 Al12 0.00(12) 34_565 34_565
Si12 Mn4 Al12 120.0 30_655 34_565
Si12 Mn4 Al12 120.0 26_556 34_565
Si12 Mn4 Al12 120.0 34_565 30_655
Si12 Mn4 Al12 0.0(2) 30_655 30_655
Si12 Mn4 Al12 120.0 26_556 30_655
Al12 Mn4 Al12 120.0 34_565 30_655
Si12 Mn4 Al12 120.0 34_565 26_556
Si12 Mn4 Al12 120.0 30_655 26_556
Si12 Mn4 Al12 0.0(2) 26_556 26_556
Al12 Mn4 Al12 120.0 34_565 26_556
Al12 Mn4 Al12 120.0 30_655 26_556
Si12 Mn4 Al6 65.46(9) 34_565 .
Si12 Mn4 Al6 148.65(9) 30_655 .
Si12 Mn4 Al6 63.99(9) 26_556 .
Al12 Mn4 Al6 65.46(9) 34_565 .
Al12 Mn4 Al6 148.65(9) 30_655 .
Al12 Mn4 Al6 63.99(9) 26_556 .
Si12 Mn4 Al6 148.65(9) 34_565 19
Si12 Mn4 Al6 65.46(9) 30_655 19
Si12 Mn4 Al6 63.99(9) 26_556 19
Al12 Mn4 Al6 148.65(9) 34_565 19
Al12 Mn4 Al6 65.46(9) 30_655 19
Al12 Mn4 Al6 63.99(9) 26_556 19
Al6 Mn4 Al6 127.97(18) . 19
Si12 Mn4 Al6 63.99(9) 34_565 24
Si12 Mn4 Al6 148.65(9) 30_655 24
Si12 Mn4 Al6 65.46(9) 26_556 24
Al12 Mn4 Al6 63.99(9) 34_565 24
Al12 Mn4 Al6 148.65(9) 30_655 24
Al12 Mn4 Al6 65.46(9) 26_556 24
Al6 Mn4 Al6 62.71(18) . 24
Al6 Mn4 Al6 95.40(12) 19 24
Si12 Mn4 Si6 148.65(9) 34_565 5
Si12 Mn4 Si6 63.99(9) 30_655 5
Si12 Mn4 Si6 65.46(9) 26_556 5
Al12 Mn4 Si6 148.65(9) 34_565 5
Al12 Mn4 Si6 63.99(9) 30_655 5
Al12 Mn4 Si6 65.46(9) 26_556 5
Al6 Mn4 Si6 95.40(12) . 5
Al6 Mn4 Si6 62.71(18) 19 5
Al6 Mn4 Si6 130.91(18) 24 5
Si12 Mn4 Si6 63.99(9) 34_565 9
Si12 Mn4 Si6 65.46(9) 30_655 9
Si12 Mn4 Si6 148.65(9) 26_556 9
Al12 Mn4 Si6 63.99(9) 34_565 9
Al12 Mn4 Si6 65.46(9) 30_655 9
Al12 Mn4 Si6 148.65(9) 26_556 9
Al6 Mn4 Si6 95.40(12) . 9
Al6 Mn4 Si6 130.91(18) 19 9
Al6 Mn4 Si6 127.97(18) 24 9
Si6 Mn4 Si6 95.40(12) 5 9
Si4 Mn3 Al4 0.00(19) 34_565 34_565
Si4 Mn3 Si4 131.2(2) 34_565 39_666
Al4 Mn3 Si4 131.2(2) 34_565 39_666
Si4 Mn3 Al4 131.2(2) 34_565 39_666
Al4 Mn3 Al4 131.2(2) 34_565 39_666
Si4 Mn3 Al4 0.0(2) 39_666 39_666
Si4 Mn3 Si10 101.79(15) 34_565 34_565
Al4 Mn3 Si10 101.79(15) 34_565 34_565
Si4 Mn3 Si10 118.90(16) 39_666 34_565
Al4 Mn3 Si10 118.90(16) 39_666 34_565
Si4 Mn3 Al10 101.79(15) 34_565 34_565
Al4 Mn3 Al10 101.79(15) 34_565 34_565
Si4 Mn3 Al10 118.90(16) 39_666 34_565
Al4 Mn3 Al10 118.90(16) 39_666 34_565
Si10 Mn3 Al10 0.0(4) 34_565 34_565
Si4 Mn3 Si10 118.90(16) 34_565 14
Al4 Mn3 Si10 118.90(16) 34_565 14
Si4 Mn3 Si10 101.79(15) 39_666 14
Al4 Mn3 Si10 101.79(15) 39_666 14
Si10 Mn3 Si10 67.4(3) 34_565 14
Al10 Mn3 Si10 67.4(3) 34_565 14
Si4 Mn3 Al10 118.90(16) 34_565 14
Al4 Mn3 Al10 118.90(16) 34_565 14
Si4 Mn3 Al10 101.79(15) 39_666 14
Al4 Mn3 Al10 101.79(15) 39_666 14
Si10 Mn3 Al10 67.4(3) 34_565 14
Al10 Mn3 Al10 67.4(3) 34_565 14
Si10 Mn3 Al10 0.0(2) 14 14
Si4 Mn3 Si5 64.76(12) 34_565 39_666
Al4 Mn3 Si5 64.76(12) 34_565 39_666
Si4 Mn3 Si5 109.20(12) 39_666 39_666
Al4 Mn3 Si5 109.20(12) 39_666 39_666
Si10 Mn3 Si5 121.07(17) 34_565 39_666
Al10 Mn3 Si5 121.07(17) 34_565 39_666
Si10 Mn3 Si5 71.35(16) 14 39_666
Al10 Mn3 Si5 71.35(16) 14 39_666
Si4 Mn3 Al5 64.76(12) 34_565 39_666
Al4 Mn3 Al5 64.76(12) 34_565 39_666
Si4 Mn3 Al5 109.20(12) 39_666 39_666
Al4 Mn3 Al5 109.20(12) 39_666 39_666
Si10 Mn3 Al5 121.07(17) 34_565 39_666
Al10 Mn3 Al5 121.07(17) 34_565 39_666
Si10 Mn3 Al5 71.35(16) 14 39_666
Al10 Mn3 Al5 71.35(16) 14 39_666
Si5 Mn3 Al5 0.0(2) 39_666 39_666
Si4 Mn3 Al5 109.20(12) 34_565 34_565
Al4 Mn3 Al5 109.20(12) 34_565 34_565
Si4 Mn3 Al5 64.76(12) 39_666 34_565
Al4 Mn3 Al5 64.76(12) 39_666 34_565
Si10 Mn3 Al5 71.35(16) 34_565 34_565
Al10 Mn3 Al5 71.35(16) 34_565 34_565
Si10 Mn3 Al5 121.07(17) 14 34_565
Al10 Mn3 Al5 121.07(17) 14 34_565
Si5 Mn3 Al5 166.4(2) 39_666 34_565
Al5 Mn3 Al5 166.4(2) 39_666 34_565
Si4 Mn3 Si5 109.20(12) 34_565 34_565
Al4 Mn3 Si5 109.20(12) 34_565 34_565
Si4 Mn3 Si5 64.76(12) 39_666 34_565
Al4 Mn3 Si5 64.76(12) 39_666 34_565
Si10 Mn3 Si5 71.35(16) 34_565 34_565
Al10 Mn3 Si5 71.35(16) 34_565 34_565
Si10 Mn3 Si5 121.07(17) 14 34_565
Al10 Mn3 Si5 121.07(17) 14 34_565
Si5 Mn3 Si5 166.4(2) 39_666 34_565
Al5 Mn3 Si5 166.4(2) 39_666 34_565
Al5 Mn3 Si5 0.00(5) 34_565 34_565
Si14 Mn5 Si14 180.000(1) 45_666 21_455
Si14 Mn5 Al14 0.000(1) 45_666 45_666
Si14 Mn5 Al14 180.000(1) 21_455 45_666
Si14 Mn5 Al14 180.000(1) 45_666 21_455
Si14 Mn5 Al14 0.000(1) 21_455 21_455
Al14 Mn5 Al14 180.000(1) 45_666 21_455
Si14 Mn5 Si8 90.000(1) 45_666 46_666
Si14 Mn5 Si8 90.000(1) 21_455 46_666
Al14 Mn5 Si8 90.000(1) 45_666 46_666
Al14 Mn5 Si8 90.000(1) 21_455 46_666
Si14 Mn5 Si8 90.000(1) 45_666 22_455
Si14 Mn5 Si8 90.000(1) 21_455 22_455
Al14 Mn5 Si8 90.000(1) 45_666 22_455
Al14 Mn5 Si8 90.000(1) 21_455 22_455
Si8 Mn5 Si8 180.0 46_666 22_455
Si14 Mn5 Al8 90.000(1) 45_666 46_666
Si14 Mn5 Al8 90.000(1) 21_455 46_666
Al14 Mn5 Al8 90.000(1) 45_666 46_666
Al14 Mn5 Al8 90.000(1) 21_455 46_666
Si8 Mn5 Al8 0.00(17) 46_666 46_666
Si8 Mn5 Al8 180.0 22_455 46_666
Si14 Mn5 Al8 90.000(1) 45_666 22_455
Si14 Mn5 Al8 90.000(1) 21_455 22_455
Al14 Mn5 Al8 90.000(1) 45_666 22_455
Al14 Mn5 Al8 90.000(1) 21_455 22_455
Si8 Mn5 Al8 180.0 46_666 22_455
Si8 Mn5 Al8 0.00(17) 22_455 22_455
Al8 Mn5 Al8 180.0 46_666 22_455
Si14 Mn5 Al8 90.0 45_666 21_455
Si14 Mn5 Al8 90.0 21_455 21_455
Al14 Mn5 Al8 90.0 45_666 21_455
Al14 Mn5 Al8 90.0 21_455 21_455
Si8 Mn5 Al8 85.1(2) 46_666 21_455
Si8 Mn5 Al8 94.9(2) 22_455 21_455
Al8 Mn5 Al8 85.1(2) 46_666 21_455
Al8 Mn5 Al8 94.9(2) 22_455 21_455
Si14 Mn5 Si8 90.0 45_666 21_455
Si14 Mn5 Si8 90.0 21_455 21_455
Al14 Mn5 Si8 90.0 45_666 21_455
Al14 Mn5 Si8 90.0 21_455 21_455
Si8 Mn5 Si8 85.1(2) 46_666 21_455
Si8 Mn5 Si8 94.9(2) 22_455 21_455
Al8 Mn5 Si8 85.1(2) 46_666 21_455
Al8 Mn5 Si8 94.9(2) 22_455 21_455
Al8 Mn5 Si8 0.00(17) 21_455 21_455
Si14 Mn5 Si8 90.0 45_666 45_666
Si14 Mn5 Si8 90.0 21_455 45_666
Al14 Mn5 Si8 90.0 45_666 45_666
Al14 Mn5 Si8 90.0 21_455 45_666
Si8 Mn5 Si8 94.9(2) 46_666 45_666
Si8 Mn5 Si8 85.1(2) 22_455 45_666
Al8 Mn5 Si8 94.9(2) 46_666 45_666
Al8 Mn5 Si8 85.1(2) 22_455 45_666
Al8 Mn5 Si8 180.000(1) 21_455 45_666
Si8 Mn5 Si8 180.000(1) 21_455 45_666
Si14 Mn5 Al8 90.0 45_666 45_666
Si14 Mn5 Al8 90.0 21_455 45_666
Al14 Mn5 Al8 90.0 45_666 45_666
Al14 Mn5 Al8 90.0 21_455 45_666
Si8 Mn5 Al8 94.9(2) 46_666 45_666
Si8 Mn5 Al8 85.1(2) 22_455 45_666
Al8 Mn5 Al8 94.9(2) 46_666 45_666
Al8 Mn5 Al8 85.1(2) 22_455 45_666
Al8 Mn5 Al8 180.000(1) 21_455 45_666
Si8 Mn5 Al8 180.000(1) 21_455 45_666
Si8 Mn5 Al8 0.00(17) 45_666 45_666
Mn2 Al1 Mn2 117.68(15) 14 .
Mn2 Al1 Si1 59.61(17) 14 14
Mn2 Al1 Si1 58.43(16) . 14
Mn2 Al1 Al1 59.61(17) 14 14
Mn2 Al1 Al1 58.43(16) . 14
Si1 Al1 Al1 0.000(5) 14 14
Mn2 Al1 Si4 56.25(13) 14 14
Mn2 Al1 Si4 118.02(16) . 14
Si1 Al1 Si4 90.25(16) 14 14
Al1 Al1 Si4 90.25(16) 14 14
Mn2 Al1 Al4 56.25(13) 14 14
Mn2 Al1 Al4 118.02(16) . 14
Si1 Al1 Al4 90.25(16) 14 14
Al1 Al1 Al4 90.25(16) 14 14
Si4 Al1 Al4 0.0(2) 14 14
Mn2 Al1 Si14 110.18(16) 14 9
Mn2 Al1 Si14 114.32(16) . 9
Si1 Al1 Si14 131.21(14) 14 9
Al1 Al1 Si14 131.21(14) 14 9
Si4 Al1 Si14 125.42(18) 14 9
Al4 Al1 Si14 125.42(18) 14 9
Mn2 Al1 Al14 110.18(16) 14 9
Mn2 Al1 Al14 114.32(16) . 9
Si1 Al1 Al14 131.21(14) 14 9
Al1 Al1 Al14 131.21(14) 14 9
Si4 Al1 Al14 125.42(18) 14 9
Al4 Al1 Al14 125.42(18) 14 9
Si14 Al1 Al14 0.0(2) 9 9
Mn2 Al1 Al1 131.00(10) 14 28
Mn2 Al1 Al1 56.38(9) . 28
Si1 Al1 Al1 91.16(13) 14 28
Al1 Al1 Al1 91.16(13) 14 28
Si4 Al1 Al1 171.68(12) 14 28
Al4 Al1 Al1 171.68(12) 14 28
Si14 Al1 Al1 58.55(10) 9 28
Al14 Al1 Al1 58.55(10) 9 28
Mn2 Al1 Si1 131.00(10) 14 28
Mn2 Al1 Si1 56.38(9) . 28
Si1 Al1 Si1 91.16(13) 14 28
Al1 Al1 Si1 91.16(13) 14 28
Si4 Al1 Si1 171.68(12) 14 28
Al4 Al1 Si1 171.68(12) 14 28
Si14 Al1 Si1 58.55(10) 9 28
Al14 Al1 Si1 58.55(10) 9 28
Al1 Al1 Si1 0.0(2) 28 28
Mn2 Al1 Al3 122.80(17) 14 .
Mn2 Al1 Al3 54.99(13) . .
Si1 Al1 Al3 92.26(17) 14 .
Al1 Al1 Al3 92.26(17) 14 .
Si4 Al1 Al3 77.55(14) 14 .
Al4 Al1 Al3 77.55(14) 14 .
Si14 Al1 Al3 124.34(18) 9 .
Al14 Al1 Al3 124.34(18) 9 .
Al1 Al1 Al3 94.20(11) 28 .
Si1 Al1 Al3 94.20(11) 28 .
Mn1 Al2 Mn1 134.88(19) 9 .
Mn1 Al2 Al13 68.53(11) 9 .
Mn1 Al2 Al13 68.14(11) . .
Mn1 Al2 Al9 135.6(2) 9 .
Mn1 Al2 Al9 59.34(13) . .
Al13 Al2 Al9 116.41(19) . .
Mn1 Al2 Al3 62.23(14) 9 .
Mn1 Al2 Al3 131.44(18) . .
Al13 Al2 Al3 92.52(19) . .
Al9 Al2 Al3 149.4(2) . .
Mn1 Al2 Al11 58.46(12) 9 .
Mn1 Al2 Al11 145.9(2) . .
Al13 Al2 Al11 122.39(17) . .
Al9 Al2 Al11 89.53(19) . .
Al3 Al2 Al11 82.34(19) . .
Mn1 Al2 Si2 114.84(10) 9 28
Mn1 Al2 Si2 107.00(10) . 28
Al13 Al2 Si2 172.97(14) . 28
Al9 Al2 Si2 56.71(11) . 28
Al3 Al2 Si2 94.51(13) . 28
Al11 Al2 Si2 58.62(10) . 28
Mn1 Al2 Al2 114.84(10) 9 28
Mn1 Al2 Al2 107.00(10) . 28
Al13 Al2 Al2 172.97(14) . 28
Al9 Al2 Al2 56.71(11) . 28
Al3 Al2 Al2 94.51(13) . 28
Al11 Al2 Al2 58.62(10) . 28
Si2 Al2 Al2 0.0(2) 28 28
Mn2 Al3 Al2 119.34(19) . .
Mn2 Al3 Mn1 157.31(19) . 9
Al2 Al3 Mn1 56.44(13) . 9
Mn2 Al3 Si12 100.25(17) . 34_565
Al2 Al3 Si12 105.07(18) . 34_565
Mn1 Al3 Si12 102.30(16) 9 34_565
Mn2 Al3 Al12 100.25(17) . 34_565
Al2 Al3 Al12 105.07(18) . 34_565
Mn1 Al3 Al12 102.30(16) 9 34_565
Si12 Al3 Al12 0.0 34_565 34_565
Mn2 Al3 Al4 55.53(13) . .
Al2 Al3 Al4 100.13(17) . .
Mn1 Al3 Al4 144.00(19) 9 .
Si12 Al3 Al4 54.02(12) 34_565 .
Al12 Al3 Al4 54.02(12) 34_565 .
Mn2 Al3 Al1 56.36(13) . .
Al2 Al3 Al1 170.6(2) . .
Mn1 Al3 Al1 123.62(17) 9 .
Si12 Al3 Al1 84.24(16) 34_565 .
Al12 Al3 Al1 84.24(16) 34_565 .
Al4 Al3 Al1 84.13(16) . .
Mn2 Al3 Si5 123.87(18) . 9
Al2 Al3 Si5 112.9(2) . 9
Mn1 Al3 Si5 56.59(12) 9 9
Si12 Al3 Si5 84.40(13) 34_565 9
Al12 Al3 Si5 84.40(13) 34_565 9
Al4 Al3 Si5 132.77(19) . 9
Al1 Al3 Si5 68.80(14) . 9
Mn2 Al3 Al5 123.87(18) . 9
Al2 Al3 Al5 112.9(2) . 9
Mn1 Al3 Al5 56.59(12) 9 9
Si12 Al3 Al5 84.40(13) 34_565 9
Al12 Al3 Al5 84.40(13) 34_565 9
Al4 Al3 Al5 132.77(19) . 9
Al1 Al3 Al5 68.80(14) . 9
Si5 Al3 Al5 0.00(17) 9 9
Mn2 Al4 Si12 108.21(17) . 34_565
Mn2 Al4 Al12 108.21(17) . 34_565
Si12 Al4 Al12 0.0 34_565 34_565
Mn2 Al4 Mn3 141.87(18) . 31_556
Si12 Al4 Mn3 108.20(17) 34_565 31_556
Al12 Al4 Mn3 108.20(17) 34_565 31_556
Mn2 Al4 Si1 58.49(13) . 14
Si12 Al4 Si1 92.28(17) 34_565 14
Al12 Al4 Si1 92.28(17) 34_565 14
Mn3 Al4 Si1 130.34(17) 31_556 14
Mn2 Al4 Al1 58.49(13) . 14
Si12 Al4 Al1 92.28(17) 34_565 14
Al12 Al4 Al1 92.28(17) 34_565 14
Mn3 Al4 Al1 130.34(17) 31_556 14
Si1 Al4 Al1 0.0(2) 14 14
Mn2 Al4 Al3 57.35(13) . .
Si12 Al4 Al3 61.78(12) 34_565 .
Al12 Al4 Al3 61.78(12) 34_565 .
Mn3 Al4 Al3 136.53(17) 31_556 .
Si1 Al4 Al3 93.09(17) 14 .
Al1 Al4 Al3 93.09(17) 14 .
Mn2 Al4 Si5 128.01(17) . 24
Si12 Al4 Si5 93.07(14) 34_565 24
Al12 Al4 Si5 93.07(14) 34_565 24
Mn3 Al4 Si5 60.31(11) 31_556 24
Si1 Al4 Si5 74.24(15) 14 24
Al1 Al4 Si5 74.24(15) 14 24
Al3 Al4 Si5 151.80(19) . 24
Mn2 Al4 Al5 128.01(17) . 24
Si12 Al4 Al5 93.07(14) 34_565 24
Al12 Al4 Al5 93.07(14) 34_565 24
Mn3 Al4 Al5 60.31(11) 31_556 24
Si1 Al4 Al5 74.24(15) 14 24
Al1 Al4 Al5 74.24(15) 14 24
Al3 Al4 Al5 151.80(19) . 24
Si5 Al4 Al5 0.00(9) 24 24
Mn2 Al4 Al6 127.70(18) . .
Si12 Al4 Al6 63.31(14) 34_565 .
Al12 Al4 Al6 63.31(14) 34_565 .
Mn3 Al4 Al6 62.46(13) 31_556 .
Si1 Al4 Al6 155.57(19) 14 .
Al1 Al4 Al6 155.57(19) 14 .
Al3 Al4 Al6 76.86(15) . .
Si5 Al4 Al6 104.29(16) 24 .
Al5 Al4 Al6 104.29(16) 24 .
Mn3 Al5 Al6 62.09(14) 31_556 .
Mn3 Al5 Mn1 120.21(15) 31_556 .
Al6 Al5 Mn1 60.65(13) . .
Mn3 Al5 Al8 111.6(2) 31_556 .
Al6 Al5 Al8 159.2(2) . .
Mn1 Al5 Al8 115.42(19) . .
Mn3 Al5 Al7 133.87(18) 31_556 .
Al6 Al5 Al7 108.6(2) . .
Mn1 Al5 Al7 56.74(13) . .
Al8 Al5 Al7 60.02(17) . .
Mn3 Al5 Si4 54.93(11) 31_556 24
Al6 Al5 Si4 71.82(15) . 24
Mn1 Al5 Si4 117.97(17) . 24
Al8 Al5 Si4 122.51(19) . 24
Al7 Al5 Si4 170.7(2) . 24
Mn3 Al5 Al4 54.93(11) 31_556 24
Al6 Al5 Al4 71.82(15) . 24
Mn1 Al5 Al4 117.97(17) . 24
Al8 Al5 Al4 122.51(19) . 24
Al7 Al5 Al4 170.7(2) . 24
Si4 Al5 Al4 0.00(16) 24 24
Mn3 Al5 Si3 119.70(17) 31_556 5
Al6 Al5 Si3 72.82(15) . 5
Mn1 Al5 Si3 55.29(12) . 5
Al8 Al5 Si3 123.44(19) . 5
Al7 Al5 Si3 96.17(17) . 5
Si4 Al5 Si3 74.93(15) 24 5
Al4 Al5 Si3 74.93(15) 24 5
Mn3 Al5 Al3 119.70(17) 31_556 5
Al6 Al5 Al3 72.82(15) . 5
Mn1 Al5 Al3 55.29(12) . 5
Al8 Al5 Al3 123.44(19) . 5
Al7 Al5 Al3 96.17(17) . 5
Si4 Al5 Al3 74.93(15) 24 5
Al4 Al5 Al3 74.93(15) 24 5
Si3 Al5 Al3 0.0(2) 5 5
Al5 Al6 Mn1 59.76(13) . .
Al5 Al6 Al13 121.8(2) . .
Mn1 Al6 Al13 63.97(16) . .
Al5 Al6 Mn4 142.98(18) . .
Mn1 Al6 Mn4 120.68(17) . .
Al13 Al6 Mn4 62.67(16) . .
Al5 Al6 Si12 90.33(18) . 26_556
Mn1 Al6 Si12 100.35(15) . 26_556
Al13 Al6 Si12 86.07(16) . 26_556
Mn4 Al6 Si12 52.65(12) . 26_556
Al5 Al6 Al12 90.33(18) . 26_556
Mn1 Al6 Al12 100.35(15) . 26_556
Al13 Al6 Al12 86.07(16) . 26_556
Mn4 Al6 Al12 52.65(12) . 26_556
Si12 Al6 Al12 0.0(3) 26_556 26_556
Al5 Al6 Mn3 58.80(13) . 31_556
Mn1 Al6 Mn3 116.22(15) . 31_556
Al13 Al6 Mn3 178.38(19) . 31_556
Mn4 Al6 Mn3 117.87(15) . 31_556
Si12 Al6 Mn3 95.45(14) 26_556 31_556
Al12 Al6 Mn3 95.45(14) 26_556 31_556
Al5 Al6 Si12 152.4(2) . 34_565
Mn1 Al6 Si12 142.01(17) . 34_565
Al13 Al6 Si12 84.99(15) . 34_565
Mn4 Al6 Si12 52.07(11) . 34_565
Si12 Al6 Si12 98.6(2) 26_556 34_565
Al12 Al6 Si12 98.6(2) 26_556 34_565
Mn3 Al6 Si12 94.21(14) 31_556 34_565
Al5 Al6 Al12 152.4(2) . 34_565
Mn1 Al6 Al12 142.01(17) . 34_565
Al13 Al6 Al12 84.99(15) . 34_565
Mn4 Al6 Al12 52.07(11) . 34_565
Si12 Al6 Al12 98.6(2) 26_556 34_565
Al12 Al6 Al12 98.6(2) 26_556 34_565
Mn3 Al6 Al12 94.21(14) 31_556 34_565
Si12 Al6 Al12 0.00(6) 34_565 34_565
Al9 Al7 Mn1 59.28(12) . 28
Al9 Al7 Mn1 59.28(12) . .
Mn1 Al7 Mn1 113.9(2) 28 .
Al9 Al7 Al8 169.0(3) . .
Mn1 Al7 Al8 117.69(13) 28 .
Mn1 Al7 Al8 117.69(13) . .
Al9 Al7 Al5 114.74(19) . .
Mn1 Al7 Al5 135.7(2) 28 .
Mn1 Al7 Al5 60.14(11) . .
Al8 Al7 Al5 58.95(14) . .
Al9 Al7 Si5 114.74(19) . 28
Mn1 Al7 Si5 60.14(11) 28 28
Mn1 Al7 Si5 135.7(2) . 28
Al8 Al7 Si5 58.95(14) . 28
Al5 Al7 Si5 92.7(2) . 28
Al9 Al7 Al5 114.74(19) . 28
Mn1 Al7 Al5 60.14(11) 28 28
Mn1 Al7 Al5 135.7(2) . 28
Al8 Al7 Al5 58.95(14) . 28
Al5 Al7 Al5 92.7(2) . 28
Si5 Al7 Al5 0.00(19) 28 28
Al9 Al7 Er3 125.97(16) . 30
Mn1 Al7 Er3 82.15(6) 28 30
Mn1 Al7 Er3 158.21(19) . 30
Al8 Al7 Er3 61.28(13) . 30
Al5 Al7 Er3 119.3(2) . 30
Si5 Al7 Er3 64.50(11) 28 30
Al5 Al7 Er3 64.50(11) 28 30
Al9 Al7 Er3 125.97(16) . 5
Mn1 Al7 Er3 158.21(19) 28 5
Mn1 Al7 Er3 82.15(6) . 5
Al8 Al7 Er3 61.28(13) . 5
Al5 Al7 Er3 64.50(11) . 5
Si5 Al7 Er3 119.3(2) 28 5
Al5 Al7 Er3 119.3(2) 28 5
Er3 Al7 Er3 78.91(13) 30 5
Mn5 Al8 Al5 132.07(12) 21_445 .
Mn5 Al8 Si5 132.07(12) 21_445 28
Al5 Al8 Si5 95.3(2) . 28
Mn5 Al8 Al5 132.07(12) 21_445 28
Al5 Al8 Al5 95.3(2) . 28
Si5 Al8 Al5 0.00(19) 28 28
Mn5 Al8 Al7 130.0(3) 21_445 .
Al5 Al8 Al7 61.04(15) . .
Si5 Al8 Al7 61.04(15) 28 .
Al5 Al8 Al7 61.04(15) 28 .
Mn5 Al8 Er2 84.00(12) 21_445 45_666
Al5 Al8 Er2 66.58(11) . 45_666
Si5 Al8 Er2 129.5(2) 28 45_666
Al5 Al8 Er2 129.5(2) 28 45_666
Al7 Al8 Er2 127.50(13) . 45_666
Mn5 Al8 Er2 84.00(12) 21_445 22_455
Al5 Al8 Er2 129.5(2) . 22_455
Si5 Al8 Er2 66.58(11) 28 22_455
Al5 Al8 Er2 66.58(11) 28 22_455
Al7 Al8 Er2 127.50(13) . 22_455
Er2 Al8 Er2 88.74(15) 45_666 22_455
Mn5 Al8 Er3 78.00(13) 21_445 30
Al5 Al8 Er3 125.1(2) . 30
Si5 Al8 Er3 66.62(11) 28 30
Al5 Al8 Er3 66.62(11) 28 30
Al7 Al8 Er3 65.09(14) . 30
Er2 Al8 Er3 161.8(2) 45_666 30
Er2 Al8 Er3 91.78(4) 22_455 30
Mn5 Al8 Er3 78.00(13) 21_445 5
Al5 Al8 Er3 66.62(11) . 5
Si5 Al8 Er3 125.1(2) 28 5
Al5 Al8 Er3 125.1(2) 28 5
Al7 Al8 Er3 65.09(14) . 5
Er2 Al8 Er3 91.78(4) 45_666 5
Er2 Al8 Er3 161.8(2) 22_455 5
Er3 Al8 Er3 82.17(14) 30 5
Mn1 Al9 Mn1 117.3(2) 28 .
Mn1 Al9 Al7 61.17(12) 28 .
Mn1 Al9 Al7 61.17(12) . .
Mn1 Al9 Si2 58.45(12) 28 28
Mn1 Al9 Si2 114.5(2) . 28
Al7 Al9 Si2 102.4(2) . 28
Mn1 Al9 Al2 58.45(12) 28 28
Mn1 Al9 Al2 114.5(2) . 28
Al7 Al9 Al2 102.4(2) . 28
Si2 Al9 Al2 0.0(2) 28 28
Mn1 Al9 Al2 114.5(2) 28 .
Mn1 Al9 Al2 58.44(12) . .
Al7 Al9 Al2 102.4(2) . .
Si2 Al9 Al2 66.6(2) 28 .
Al2 Al9 Al2 66.6(2) 28 .
Mn1 Al9 Si15 112.53(16) 28 9
Mn1 Al9 Si15 112.53(16) . 9
Al7 Al9 Si15 115.4(3) . 9
Si2 Al9 Si15 129.6(2) 28 9
Al2 Al9 Si15 129.6(2) 28 9
Al2 Al9 Si15 129.6(2) . 9
Mn1 Al9 Al15 112.53(16) 28 9
Mn1 Al9 Al15 112.53(16) . 9
Al7 Al9 Al15 115.4(3) . 9
Si2 Al9 Al15 129.6(2) 28 9
Al2 Al9 Al15 129.6(2) 28 9
Al2 Al9 Al15 129.6(2) . 9
Si15 Al9 Al15 0.0(3) 9 9
Mn1 Al9 Si11 55.78(12) 28 30
Mn1 Al9 Si11 119.7(2) . 30
Al7 Al9 Si11 69.36(19) . 30
Si2 Al9 Si11 107.58(13) 28 30
Al2 Al9 Si11 107.58(13) 28 30
Al2 Al9 Si11 169.2(3) . 30
Si15 Al9 Si11 61.17(19) 9 30
Al15 Al9 Si11 61.17(19) 9 30
Mn1 Al9 Al11 55.78(12) 28 30
Mn1 Al9 Al11 119.7(2) . 30
Al7 Al9 Al11 69.36(19) . 30
Si2 Al9 Al11 107.58(13) 28 30
Al2 Al9 Al11 107.58(13) 28 30
Al2 Al9 Al11 169.2(3) . 30
Si15 Al9 Al11 61.17(19) 9 30
Al15 Al9 Al11 61.17(19) 9 30
Si11 Al9 Al11 0.0(3) 30 30
Mn3 Al10 Mn3 134.3(2) 31_556 8_556
Mn3 Al10 Si10 56.28(13) 31_556 45_666
Mn3 Al10 Si10 123.5(3) 8_556 45_666
Mn3 Al10 Al10 56.28(13) 31_556 45_666
Mn3 Al10 Al10 123.5(3) 8_556 45_666
Si10 Al10 Al10 0.0(2) 45_666 45_666
Mn3 Al10 Si10 123.5(3) 31_556 22_455
Mn3 Al10 Si10 56.28(13) 8_556 22_455
Si10 Al10 Si10 73.8(2) 45_666 22_455
Al10 Al10 Si10 73.8(2) 45_666 22_455
Mn3 Al10 Al10 123.5(3) 31_556 22_455
Mn3 Al10 Al10 56.28(13) 8_556 22_455
Si10 Al10 Al10 73.8(2) 45_666 22_455
Al10 Al10 Al10 73.8(2) 45_666 22_455
Si10 Al10 Al10 0.00(18) 22_455 22_455
Mn3 Al10 Al8 106.69(14) 31_556 .
Mn3 Al10 Al8 106.69(14) 8_556 .
Si10 Al10 Al8 122.8(3) 45_666 .
Al10 Al10 Al8 122.8(3) 45_666 .
Si10 Al10 Al8 122.8(3) 22_455 .
Al10 Al10 Al8 122.8(3) 22_455 .
Mn3 Al10 Er1 74.82(13) 31_556 .
Mn3 Al10 Er1 74.82(13) 8_556 .
Si10 Al10 Er1 125.99(19) 45_666 .
Al10 Al10 Er1 125.99(19) 45_666 .
Si10 Al10 Er1 125.99(19) 22_455 .
Al10 Al10 Er1 125.99(19) 22_455 .
Al8 Al10 Er1 90.10(19) . .
Mn3 Al10 Al5 56.40(10) 31_556 .
Mn3 Al10 Al5 131.2(2) 8_556 .
Si10 Al10 Al5 101.45(15) 45_666 .
Al10 Al10 Al5 101.45(15) 45_666 .
Si10 Al10 Al5 171.2(2) 22_455 .
Al10 Al10 Al5 171.2(2) 22_455 .
Al8 Al10 Al5 53.23(13) . .
Er1 Al10 Al5 62.84(13) . .
Mn3 Al10 Al5 131.2(2) 31_556 28
Mn3 Al10 Al5 56.40(10) 8_556 28
Si10 Al10 Al5 171.2(2) 45_666 28
Al10 Al10 Al5 171.2(2) 45_666 28
Si10 Al10 Al5 101.45(15) 22_455 28
Al10 Al10 Al5 101.45(15) 22_455 28
Al8 Al10 Al5 53.23(13) . 28
Er1 Al10 Al5 62.84(13) . 28
Al5 Al10 Al5 82.2(2) . 28
Mn3 Al10 Er2 152.89(19) 31_556 22_455
Mn3 Al10 Er2 72.77(6) 8_556 22_455
Si10 Al10 Er2 111.51(14) 45_666 22_455
Al10 Al10 Er2 111.51(14) 45_666 22_455
Si10 Al10 Er2 66.02(18) 22_455 22_455
Al10 Al10 Er2 66.02(18) 22_455 22_455
Al8 Al10 Er2 56.89(12) . 22_455
Er1 Al10 Er2 122.49(14) . 22_455
Al5 Al10 Er2 110.0(2) . 22_455
Al5 Al10 Er2 59.68(11) 28 22_455
Mn1 Al11 Mn1 149.4(3) 9 35
Mn1 Al11 Si2 116.1(2) 9 28
Mn1 Al11 Si2 55.63(12) 35 28
Mn1 Al11 Al2 116.1(2) 9 28
Mn1 Al11 Al2 55.63(12) 35 28
Si2 Al11 Al2 0.0(2) 28 28
Mn1 Al11 Al2 55.63(12) 9 .
Mn1 Al11 Al2 116.1(2) 35 .
Si2 Al11 Al2 62.8(2) 28 .
Al2 Al11 Al2 62.8(2) 28 .
Mn1 Al11 Si15 105.18(14) 9 5
Mn1 Al11 Si15 105.18(14) 35 5
Si2 Al11 Si15 109.6(2) 28 5
Al2 Al11 Si15 109.6(2) 28 5
Al2 Al11 Si15 109.6(2) . 5
Mn1 Al11 Al15 105.18(14) 9 5
Mn1 Al11 Al15 105.18(14) 35 5
Si2 Al11 Al15 109.6(2) 28 5
Al2 Al11 Al15 109.6(2) 28 5
Al2 Al11 Al15 109.6(2) . 5
Si15 Al11 Al15 0.0(2) 5 5
Mn1 Al11 Si9 149.5(2) 9 10
Mn1 Al11 Si9 54.79(11) 35 10
Si2 Al11 Si9 93.40(13) 28 10
Al2 Al11 Si9 93.40(13) 28 10
Al2 Al11 Si9 146.7(2) . 10
Si15 Al11 Si9 54.25(15) 5 10
Al15 Al11 Si9 54.25(15) 5 10
Mn1 Al11 Al9 149.5(2) 9 10
Mn1 Al11 Al9 54.79(11) 35 10
Si2 Al11 Al9 93.40(13) 28 10
Al2 Al11 Al9 93.40(13) 28 10
Al2 Al11 Al9 146.7(2) . 10
Si15 Al11 Al9 54.25(15) 5 10
Al15 Al11 Al9 54.25(15) 5 10
Si9 Al11 Al9 0.0(3) 10 10
Mn1 Al11 Al9 54.79(11) 9 9
Mn1 Al11 Al9 149.5(2) 35 9
Si2 Al11 Al9 146.7(2) 28 9
Al2 Al11 Al9 146.7(2) 28 9
Al2 Al11 Al9 93.40(13) . 9
Si15 Al11 Al9 54.25(15) 5 9
Al15 Al11 Al9 54.25(15) 5 9
Si9 Al11 Al9 96.4(2) 10 9
Al9 Al11 Al9 96.4(2) 10 9
Mn1 Al11 Si9 54.79(11) 9 9
Mn1 Al11 Si9 149.5(2) 35 9
Si2 Al11 Si9 146.7(2) 28 9
Al2 Al11 Si9 146.7(2) 28 9
Al2 Al11 Si9 93.40(13) . 9
Si15 Al11 Si9 54.25(15) 5 9
Al15 Al11 Si9 54.25(15) 5 9
Si9 Al11 Si9 96.4(2) 10 9
Al9 Al11 Si9 96.4(2) 10 9
Al9 Al11 Si9 0.0(3) 9 9
Mn4 Al12 Si4 122.66(12) 26_556 45_666
Mn4 Al12 Al4 122.66(12) 26_556 45_666
Si4 Al12 Al4 0.00(14) 45_666 45_666
Mn4 Al12 Si4 122.66(12) 26_556 31_556
Si4 Al12 Si4 114.7(2) 45_666 31_556
Al4 Al12 Si4 114.7(2) 45_666 31_556
Mn4 Al12 Al4 122.66(12) 26_556 31_556
Si4 Al12 Al4 114.7(2) 45_666 31_556
Al4 Al12 Al4 114.7(2) 45_666 31_556
Si4 Al12 Al4 0.00(19) 31_556 31_556
Mn4 Al12 Al3 119.47(13) 26_556 31_556
Si4 Al12 Al3 84.51(15) 45_666 31_556
Al4 Al12 Al3 84.51(15) 45_666 31_556
Si4 Al12 Al3 64.20(13) 31_556 31_556
Al4 Al12 Al3 64.20(13) 31_556 31_556
Mn4 Al12 Si3 119.47(13) 26_556 31_556
Si4 Al12 Si3 84.51(15) 45_666 31_556
Al4 Al12 Si3 84.51(15) 45_666 31_556
Si4 Al12 Si3 64.20(13) 31_556 31_556
Al4 Al12 Si3 64.20(13) 31_556 31_556
Al3 Al12 Si3 0.00(17) 31_556 31_556
Mn4 Al12 Si3 119.47(13) 26_556 45_666
Si4 Al12 Si3 64.20(13) 45_666 45_666
Al4 Al12 Si3 64.20(13) 45_666 45_666
Si4 Al12 Si3 84.51(15) 31_556 45_666
Al4 Al12 Si3 84.51(15) 31_556 45_666
Al3 Al12 Si3 121.1(3) 31_556 45_666
Si3 Al12 Si3 121.1(3) 31_556 45_666
Mn4 Al12 Al3 119.47(13) 26_556 45_666
Si4 Al12 Al3 64.20(13) 45_666 45_666
Al4 Al12 Al3 64.20(13) 45_666 45_666
Si4 Al12 Al3 84.51(15) 31_556 45_666
Al4 Al12 Al3 84.51(15) 31_556 45_666
Al3 Al12 Al3 121.1(3) 31_556 45_666
Si3 Al12 Al3 121.1(3) 31_556 45_666
Si3 Al12 Al3 0.00(9) 45_666 45_666
Mn4 Al12 Si6 63.36(13) 26_556 41_666
Si4 Al12 Si6 137.24(12) 45_666 41_666
Al4 Al12 Si6 137.24(12) 45_666 41_666
Si4 Al12 Si6 75.50(12) 31_556 41_666
Al4 Al12 Si6 75.50(12) 31_556 41_666
Al3 Al12 Si6 132.47(13) 31_556 41_666
Si3 Al12 Si6 132.47(13) 31_556 41_666
Si3 Al12 Si6 76.47(12) 45_666 41_666
Al3 Al12 Si6 76.47(12) 45_666 41_666
Mn4 Al12 Al6 63.36(13) 26_556 41_666
Si4 Al12 Al6 137.24(12) 45_666 41_666
Al4 Al12 Al6 137.24(12) 45_666 41_666
Si4 Al12 Al6 75.50(12) 31_556 41_666
Al4 Al12 Al6 75.50(12) 31_556 41_666
Al3 Al12 Al6 132.47(13) 31_556 41_666
Si3 Al12 Al6 132.47(13) 31_556 41_666
Si3 Al12 Al6 76.47(12) 45_666 41_666
Al3 Al12 Al6 76.47(12) 45_666 41_666
Si6 Al12 Al6 0.00(19) 41_666 41_666
Mn4 Al12 Al6 63.36(13) 26_556 26_556
Si4 Al12 Al6 75.50(12) 45_666 26_556
Al4 Al12 Al6 75.50(12) 45_666 26_556
Si4 Al12 Al6 137.24(12) 31_556 26_556
Al4 Al12 Al6 137.24(12) 31_556 26_556
Al3 Al12 Al6 76.47(12) 31_556 26_556
Si3 Al12 Al6 76.47(12) 31_556 26_556
Si3 Al12 Al6 132.47(13) 45_666 26_556
Al3 Al12 Al6 132.47(13) 45_666 26_556
Si6 Al12 Al6 126.7(3) 41_666 26_556
Al6 Al12 Al6 126.7(3) 41_666 26_556
Al2 Al13 Si2 97.6(2) . 9
Al2 Al13 Al2 97.6(2) . 9
Si2 Al13 Al2 0.00(16) 9 9
Al2 Al13 Si2 97.6(2) . 5
Si2 Al13 Si2 97.6(2) 9 5
Al2 Al13 Si2 97.6(2) 9 5
Al2 Al13 Al2 97.6(2) . 5
Si2 Al13 Al2 97.6(2) 9 5
Al2 Al13 Al2 97.6(2) 9 5
Si2 Al13 Al2 0.0(2) 5 5
Al2 Al13 Al6 69.93(12) . .
Si2 Al13 Al6 159.27(12) 9 .
Al2 Al13 Al6 159.27(12) 9 .
Si2 Al13 Al6 100.38(12) 5 .
Al2 Al13 Al6 100.38(12) 5 .
Al2 Al13 Si6 100.38(12) . 9
Si2 Al13 Si6 69.93(12) 9 9
Al2 Al13 Si6 69.93(12) 9 9
Si2 Al13 Si6 159.28(12) 5 9
Al2 Al13 Si6 159.28(12) 5 9
Al6 Al13 Si6 95.4(2) . 9
Al2 Al13 Al6 100.38(12) . 9
Si2 Al13 Al6 69.93(12) 9 9
Al2 Al13 Al6 69.93(12) 9 9
Si2 Al13 Al6 159.28(12) 5 9
Al2 Al13 Al6 159.28(12) 5 9
Al6 Al13 Al6 95.4(2) . 9
Si6 Al13 Al6 0.00(17) 9 9
Al2 Al13 Si6 159.27(12) . 5
Si2 Al13 Si6 100.38(12) 9 5
Al2 Al13 Si6 100.38(12) 9 5
Si2 Al13 Si6 69.93(12) 5 5
Al2 Al13 Si6 69.93(12) 5 5
Al6 Al13 Si6 95.4(2) . 5
Si6 Al13 Si6 95.4(2) 9 5
Al6 Al13 Si6 95.4(2) 9 5
Al2 Al13 Al6 159.27(12) . 5
Si2 Al13 Al6 100.38(12) 9 5
Al2 Al13 Al6 100.38(12) 9 5
Si2 Al13 Al6 69.93(12) 5 5
Al2 Al13 Al6 69.93(12) 5 5
Al6 Al13 Al6 95.4(2) . 5
Si6 Al13 Al6 95.4(2) 9 5
Al6 Al13 Al6 95.4(2) 9 5
Si6 Al13 Al6 0.0(2) 5 5
Mn5 Al14 Si1 131.27(14) 21_445 31_556
Mn5 Al14 Al1 131.27(14) 21_445 31_556
Si1 Al14 Al1 0.0(2) 31_556 31_556
Mn5 Al14 Si1 131.27(14) 21_445 6_556
Si1 Al14 Si1 62.9(2) 31_556 6_556
Al1 Al14 Si1 62.9(2) 31_556 6_556
Mn5 Al14 Si1 131.27(14) 21_445 5
Si1 Al14 Si1 65.5(2) 31_556 5
Al1 Al14 Si1 65.5(2) 31_556 5
Si1 Al14 Si1 97.5(3) 6_556 5
Mn5 Al14 Al1 131.27(14) 21_445 6_556
Si1 Al14 Al1 62.9(2) 31_556 6_556
Al1 Al14 Al1 62.9(2) 31_556 6_556
Si1 Al14 Al1 0.00(19) 6_556 6_556
Si1 Al14 Al1 97.5(3) 5 6_556
Mn5 Al14 Al1 131.27(14) 21_445 5
Si1 Al14 Al1 65.5(2) 31_556 5
Al1 Al14 Al1 65.5(2) 31_556 5
Si1 Al14 Al1 97.5(3) 6_556 5
Si1 Al14 Al1 0.0(2) 5 5
Al1 Al14 Al1 97.5(3) 6_556 5
Mn5 Al14 Si1 131.27(14) 21_445 32
Si1 Al14 Si1 97.5(3) 31_556 32
Al1 Al14 Si1 97.5(3) 31_556 32
Si1 Al14 Si1 65.5(2) 6_556 32
Si1 Al14 Si1 62.9(2) 5 32
Al1 Al14 Si1 65.5(2) 6_556 32
Al1 Al14 Si1 62.9(2) 5 32
Mn5 Al14 Al1 131.27(14) 21_445 32
Si1 Al14 Al1 97.5(3) 31_556 32
Al1 Al14 Al1 97.5(3) 31_556 32
Si1 Al14 Al1 65.5(2) 6_556 32
Si1 Al14 Al1 62.9(2) 5 32
Al1 Al14 Al1 65.5(2) 6_556 32
Al1 Al14 Al1 62.9(2) 5 32
Si1 Al14 Al1 0.00(19) 32 32
Mn5 Al14 Er3 78.98(13) 21_445 5
Si1 Al14 Er3 131.09(17) 31_556 5
Al1 Al14 Er3 131.09(17) 31_556 5
Si1 Al14 Er3 131.09(17) 6_556 5
Si1 Al14 Er3 66.10(10) 5 5
Al1 Al14 Er3 131.09(17) 6_556 5
Al1 Al14 Er3 66.10(10) 5 5
Si1 Al14 Er3 66.10(10) 32 5
Al1 Al14 Er3 66.10(10) 32 5
Mn5 Al14 Er3 78.98(13) 21_445 6_556
Si1 Al14 Er3 66.10(10) 31_556 6_556
Al1 Al14 Er3 66.10(10) 31_556 6_556
Si1 Al14 Er3 66.10(10) 6_556 6_556
Si1 Al14 Er3 131.09(17) 5 6_556
Al1 Al14 Er3 66.10(10) 6_556 6_556
Al1 Al14 Er3 131.09(17) 5 6_556
Si1 Al14 Er3 131.09(17) 32 6_556
Al1 Al14 Er3 131.09(17) 32 6_556
Er3 Al14 Er3 158.0(3) 5 6_556
Mn5 Al14 Er2 81.79(13) 21_445 46_656
Si1 Al14 Er2 127.63(17) 31_556 46_656
Al1 Al14 Er2 127.63(17) 31_556 46_656
Si1 Al14 Er2 65.03(9) 6_556 46_656
Si1 Al14 Er2 127.63(17) 5 46_656
Al1 Al14 Er2 65.03(9) 6_556 46_656
Al1 Al14 Er2 127.63(17) 5 46_656
Si1 Al14 Er2 65.03(9) 32 46_656
Al1 Al14 Er2 65.03(9) 32 46_656
Er3 Al14 Er2 88.44(4) 5 46_656
Er3 Al14 Er2 88.44(4) 6_556 46_656
Si9 Al15 Al9 0.0(2) 5 5
Si9 Al15 Si9 112.2(4) 5 6
Al9 Al15 Si9 112.2(4) 5 6
Si9 Al15 Al9 112.2(4) 5 6
Al9 Al15 Al9 112.2(4) 5 6
Si9 Al15 Al9 0.0(2) 6 6
Si9 Al15 Si11 64.58(17) 5 9
Al9 Al15 Si11 64.58(17) 5 9
Si9 Al15 Si11 64.58(17) 6 9
Al9 Al15 Si11 64.58(17) 6 9
Si9 Al15 Al11 64.58(17) 5 9
Al9 Al15 Al11 64.58(17) 5 9
Si9 Al15 Al11 64.58(17) 6 9
Al9 Al15 Al11 64.58(17) 6 9
Si11 Al15 Al11 0.0(3) 9 9
Si9 Al15 Si11 64.58(17) 5 34
Al9 Al15 Si11 64.58(17) 5 34
Si9 Al15 Si11 64.58(17) 6 34
Al9 Al15 Si11 64.58(17) 6 34
Si11 Al15 Si11 79.4(3) 9 34
Al11 Al15 Si11 79.4(3) 9 34
Si9 Al15 Al11 64.58(17) 5 34
Al9 Al15 Al11 64.58(17) 5 34
Si9 Al15 Al11 64.58(17) 6 34
Al9 Al15 Al11 64.58(17) 6 34
Si11 Al15 Al11 79.4(3) 9 34
Al11 Al15 Al11 79.4(3) 9 34
Si11 Al15 Al11 0.0(3) 34 34
Si9 Al15 Al16 123.91(19) 5 .
Al9 Al15 Al16 123.91(19) 5 .
Si9 Al15 Al16 123.91(19) 6 .
Al9 Al15 Al16 123.91(19) 6 .
Si11 Al15 Al16 140.30(16) 9 .
Al11 Al15 Al16 140.30(16) 9 .
Si11 Al15 Al16 140.30(16) 34 .
Al11 Al15 Al16 140.30(16) 34 .
Si9 Al15 Er4 135.18(12) 5 4
Al9 Al15 Er4 135.18(12) 5 4
Si9 Al15 Er4 64.81(8) 6 4
Al9 Al15 Er4 64.81(8) 6 4
Si11 Al15 Er4 129.23(17) 9 4
Al11 Al15 Er4 129.23(17) 9 4
Si11 Al15 Er4 76.04(10) 34 4
Al11 Al15 Er4 76.04(10) 34 4
Al16 Al15 Er4 75.27(14) . 4
Si9 Al15 Er4 64.81(8) 5 27
Al9 Al15 Er4 64.81(8) 5 27
Si9 Al15 Er4 135.18(12) 6 27
Al9 Al15 Er4 135.18(12) 6 27
Si11 Al15 Er4 129.23(17) 9 27
Al11 Al15 Er4 129.23(17) 9 27
Si11 Al15 Er4 76.04(10) 34 27
Al11 Al15 Er4 76.04(10) 34 27
Al16 Al15 Er4 75.27(14) . 27
Er4 Al15 Er4 86.29(7) 4 27
Si15 Al16 Si15 180.0 33 9
Si15 Al16 Si15 90.0 33 25
Si15 Al16 Si15 90.0 9 25
Si15 Al16 Al15 0.0 33 33
Si15 Al16 Al15 180.0 9 33
Si15 Al16 Al15 90.0 25 33
Si15 Al16 Al15 180.0 33 9
Si15 Al16 Al15 0.0 9 9
Si15 Al16 Al15 90.0 25 9
Al15 Al16 Al15 180.0 33 9
Si15 Al16 Al15 90.0 33 25
Si15 Al16 Al15 90.0 9 25
Si15 Al16 Al15 0.0 25 25
Al15 Al16 Al15 90.0 33 25
Al15 Al16 Al15 90.0 9 25
Si15 Al16 Si15 90.0 33 29
Si15 Al16 Si15 90.0 9 29
Si15 Al16 Si15 90.0 25 29
Al15 Al16 Si15 90.0 33 29
Al15 Al16 Si15 90.0 9 29
Al15 Al16 Si15 90.0 25 29
Si15 Al16 Si15 90.0 33 5
Si15 Al16 Si15 90.0 9 5
Si15 Al16 Si15 90.0 25 5
Al15 Al16 Si15 90.0 33 5
Al15 Al16 Si15 90.0 9 5
Al15 Al16 Si15 90.0 25 5
Si15 Al16 Si15 180.0 29 5
Si15 Al16 Al15 90.0 33 29
Si15 Al16 Al15 90.0 9 29
Si15 Al16 Al15 90.0 25 29
Al15 Al16 Al15 90.0 33 29
Al15 Al16 Al15 90.0 9 29
Al15 Al16 Al15 90.0 25 29
Si15 Al16 Al15 0.0 29 29
Si15 Al16 Al15 180.0 5 29
Si15 Al16 Al15 90.0 33 5
Si15 Al16 Al15 90.0 9 5
Si15 Al16 Al15 90.0 25 5
Al15 Al16 Al15 90.0 33 5
Al15 Al16 Al15 90.0 9 5
Al15 Al16 Al15 90.0 25 5
Si15 Al16 Al15 180.0 29 5
Si15 Al16 Al15 0.0 5 5
Al15 Al16 Al15 180.0 29 5
Si15 Al16 Al15 90.0 33 .
Si15 Al16 Al15 90.0 9 .
Si15 Al16 Al15 180.0 25 .
Al15 Al16 Al15 90.0 33 .
Al15 Al16 Al15 90.0 9 .
Al15 Al16 Al15 180.0 25 .
Si15 Al16 Al15 90.0 29 .
Si15 Al16 Al15 90.0 5 .
Al15 Al16 Al15 90.0 29 .
Al15 Al16 Al15 90.0 5 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Er1 Al4 2.825(4) .
Er1 Si4 2.825(4) 28
Er1 Al4 2.825(4) 28
Er1 Al2 2.871(4) .
Er1 Si2 2.871(4) 28
Er1 Al2 2.871(4) 28
Er1 Al10 2.926(5) .
Er1 Si5 3.054(4) 28
Er1 Al5 3.054(4) 28
Er2 Si8 2.868(4) 45_666
Er2 Al8 2.868(4) 45_666
Er2 Si8 2.868(4) 22_455
Er2 Al8 2.868(4) 22_455
Er2 Al4 2.949(4) .
Er2 Si4 2.950(4) 28
Er2 Al4 2.950(4) 28
Er2 Si5 3.014(4) 24
Er2 Al5 3.014(4) 24
Er2 Si5 3.014(4) 47_566
Er2 Al5 3.014(4) 47_566
Er3 Si8 2.873(4) 10
Er3 Al8 2.873(4) 10
Er3 Si8 2.873(4) 9
Er3 Al8 2.873(4) 9
Er3 Si14 2.8792(16) 9
Er3 Al14 2.8792(16) 9
Er3 Si7 2.972(4) 10
Er3 Al7 2.972(4) 10
Er3 Si7 2.972(4) 9
Er3 Al7 2.972(4) 9
Er3 Al1 3.018(4) 28
Er3 Si1 3.018(4) 28
Er4 Si15 2.920(2) 9
Er4 Si15 2.920(2) 5
Er4 Al15 2.920(2) 9
Er4 Al15 2.920(2) 5
Er4 Al15 2.920(2) .
Er4 Si9 2.936(4) 9
Er4 Si9 2.936(4) 5
Er4 Al9 2.936(4) 9
Er4 Al9 2.936(4) 5
Er4 Al9 2.936(4) .
Mn1 Si2 2.403(4) 5
Mn1 Al2 2.403(4) 5
Mn1 Al2 2.428(4) .
Mn1 Al9 2.451(3) .
Mn1 Si11 2.481(2) 5
Mn1 Al11 2.481(2) 5
Mn1 Al7 2.498(3) .
Mn1 Si3 2.551(5) 5
Mn1 Al3 2.551(5) 5
Mn2 Al4 2.399(4) .
Mn2 Si4 2.399(4) 28
Mn2 Al4 2.399(4) 28
Mn2 Si3 2.450(5) 28
Mn2 Al3 2.450(5) 28
Mn2 Al3 2.450(5) .
Mn2 Si1 2.460(5) 14
Mn2 Al1 2.460(5) 14
Mn2 Si1 2.460(5) 40_566
Mn2 Al1 2.460(5) 40_566
Mn4 Si12 2.330(5) 34_565
Mn4 Si12 2.330(5) 30_655
Mn4 Si12 2.330(5) 26_556
Mn4 Al12 2.330(5) 34_565
Mn4 Al12 2.330(5) 30_655
Mn4 Al12 2.330(5) 26_556
Mn4 Al6 2.619(4) .
Mn4 Al6 2.619(4) 19
Mn4 Al6 2.619(4) 24
Mn4 Si6 2.619(4) 5
Mn4 Si6 2.619(4) 9
Mn3 Si4 2.429(4) 34_565
Mn3 Al4 2.429(4) 34_565
Mn3 Si4 2.429(4) 39_666
Mn3 Al4 2.429(4) 39_666
Mn3 Si10 2.447(3) 34_565
Mn3 Al10 2.447(3) 34_565
Mn3 Si10 2.447(3) 14
Mn3 Al10 2.447(3) 14
Mn3 Si5 2.578(4) 39_666
Mn3 Al5 2.578(4) 39_666
Mn3 Al5 2.578(4) 34_565
Mn3 Si5 2.578(4) 34_565
Mn5 Si14 2.438(7) 45_666
Mn5 Si14 2.438(7) 21_455
Mn5 Al14 2.438(7) 45_666
Mn5 Al14 2.438(7) 21_455
Mn5 Si8 2.509(5) 46_666
Mn5 Si8 2.509(5) 22_455
Mn5 Al8 2.509(5) 46_666
Mn5 Al8 2.509(5) 22_455
Mn5 Al8 2.509(5) 21_455
Mn5 Si8 2.509(5) 21_455
Mn5 Si8 2.509(5) 45_666
Mn5 Al8 2.509(5) 45_666
Al1 Mn2 2.460(5) 14
Al1 Si1 2.548(7) 14
Al1 Al1 2.548(7) 14
Al1 Si4 2.620(5) 14
Al1 Al4 2.620(5) 14
Al1 Si14 2.643(6) 9
Al1 Al14 2.643(6) 9
Al1 Al1 2.758(8) 28
Al1 Si1 2.758(8) 28
Al1 Al3 2.786(6) .
Al2 Mn1 2.403(4) 9
Al2 Al13 2.518(5) .
Al2 Al9 2.521(6) .
Al2 Al3 2.530(5) .
Al2 Al11 2.657(6) .
Al2 Si2 2.767(8) 28
Al2 Al2 2.767(8) 28
Al3 Mn1 2.551(5) 9
Al3 Si12 2.624(4) 34_565
Al3 Al12 2.624(4) 34_565
Al3 Al4 2.681(5) .
Al3 Si5 2.880(6) 9
Al3 Al5 2.880(6) 9
Al4 Si12 2.410(4) 34_565
Al4 Al12 2.410(4) 34_565
Al4 Mn3 2.429(4) 31_556
Al4 Si1 2.621(5) 14
Al4 Al1 2.621(5) 14
Al4 Si5 2.684(5) 24
Al4 Al5 2.684(5) 24
Al4 Al6 2.690(5) .
Al5 Mn3 2.578(4) 31_556
Al5 Al6 2.587(5) .
Al5 Al8 2.609(5) .
Al5 Al7 2.665(5) .
Al5 Si4 2.684(5) 24
Al5 Al4 2.684(5) 24
Al5 Si3 2.880(6) 5
Al5 Al3 2.880(6) 5
Al6 Al13 2.619(6) .
Al6 Si12 2.634(4) 26_556
Al6 Al12 2.634(4) 26_556
Al6 Mn3 2.663(5) 31_556
Al6 Si12 2.687(4) 34_565
Al6 Al12 2.687(4) 34_565
Al7 Al9 2.458(7) .
Al7 Mn1 2.498(3) 28
Al7 Al8 2.638(7) .
Al7 Si5 2.665(5) 28
Al7 Al5 2.665(5) 28
Al7 Er3 2.972(4) 30
Al7 Er3 2.972(4) 5
Al8 Mn5 2.509(5) 21_445
Al8 Si5 2.609(5) 28
Al8 Al5 2.609(5) 28
Al8 Er2 2.868(4) 45_666
Al8 Er2 2.868(4) 22_455
Al8 Er3 2.873(4) 30
Al8 Er3 2.873(4) 5
Al9 Mn1 2.451(3) 28
Al9 Si2 2.521(6) 28
Al9 Al2 2.521(6) 28
Al9 Si15 2.524(7) 9
Al9 Al15 2.524(7) 9
Al9 Si11 2.809(6) 30
Al9 Al11 2.809(6) 30
Al10 Mn3 2.448(3) 31_556
Al10 Mn3 2.448(3) 8_556
Al10 Si10 2.717(9) 45_666
Al10 Al10 2.717(9) 45_666
Al10 Si10 2.717(9) 22_455
Al10 Al10 2.717(9) 22_455
Al10 Al5 2.933(6) 28
Al10 Er2 3.116(4) 22_455
Al11 Mn1 2.481(2) 9
Al11 Mn1 2.481(2) 35
Al11 Si2 2.657(6) 28
Al11 Al2 2.657(6) 28
Al11 Si15 2.725(8) 5
Al11 Al15 2.725(8) 5
Al11 Si9 2.809(6) 10
Al11 Al9 2.809(6) 10
Al11 Al9 2.809(6) 9
Al11 Si9 2.809(6) 9
Al12 Mn4 2.330(5) 26_556
Al12 Si4 2.409(4) 45_666
Al12 Al4 2.409(4) 45_666
Al12 Si4 2.409(4) 31_556
Al12 Al4 2.409(4) 31_556
Al12 Al3 2.624(5) 31_556
Al12 Si3 2.624(5) 31_556
Al12 Si3 2.624(5) 45_666
Al12 Al3 2.624(5) 45_666
Al12 Si6 2.634(4) 41_666
Al12 Al6 2.634(4) 41_666
Al12 Al6 2.634(4) 26_556
Al13 Si2 2.518(5) 9
Al13 Al2 2.518(5) 9
Al13 Si2 2.518(5) 5
Al13 Al2 2.518(5) 5
Al13 Si6 2.619(6) 9
Al13 Al6 2.619(6) 9
Al13 Si6 2.619(6) 5
Al13 Al6 2.619(6) 5
Al14 Mn5 2.438(7) 21_445
Al14 Si1 2.643(6) 31_556
Al14 Al1 2.643(6) 31_556
Al14 Si1 2.643(6) 6_556
Al14 Si1 2.643(6) 5
Al14 Al1 2.643(6) 6_556
Al14 Al1 2.643(6) 5
Al14 Si1 2.643(6) 32
Al14 Al1 2.643(6) 32
Al14 Er3 2.8792(16) 5
Al14 Er3 2.8792(16) 6_556
Al14 Er2 3.0300(13) 46_656
Al15 Si9 2.524(7) 5
Al15 Al9 2.524(7) 5
Al15 Si9 2.524(7) 6
Al15 Al9 2.524(7) 6
Al15 Si11 2.725(8) 9
Al15 Al11 2.725(8) 9
Al15 Si11 2.725(8) 34
Al15 Al11 2.725(8) 34
Al15 Al16 2.739(7) .
Al15 Er4 2.920(2) 4
Al15 Er4 2.920(2) 27
Al16 Si15 2.739(7) 33
Al16 Si15 2.739(7) 9
Al16 Si15 2.739(7) 25
Al16 Al15 2.739(7) 33
Al16 Al15 2.739(7) 9
Al16 Al15 2.739(7) 25
Al16 Si15 2.739(7) 29
Al16 Si15 2.739(7) 5
Al16 Al15 2.739(7) 29
Al16 Al15 2.739(7) 5
